Vol. 128 (2015) No. 4 ACTA PHYSICA POLONICA A Proceedings of the International Symposium on Physics of Materials (ISPMA13) Interparticle Neck Connections in Innovative Insulated Iron Powder Compounds R. Bidulský a, * a b b c , J. Bidulská , R. de Oro , E. Hryha , M. Maccarini , I. Forno c d and M. Actis Grande a Technical University of Ko²ice, Faculty of Metallurgy, Department of Metals Forming, Letná 9, 042 00 Ko²ice, Slovakia b Chalmers University of Technology, Department of Materials and Manufacturing Technology, Rannvagen 2, 412 96 Göteborg, Sweden c d Consorzio Prometeo, Viale T. Michel 5, 15121 Alessandria, Italy Politecnico di Torino, Department of Applied Science and Technology, Viale T. Michel 5, 15121 Alessandria, Italy Goal of the present paper is the analysis of the interparticle neck connections in a system made of insulated iron powder compounds with dierent additions of an AlMgSiCu alloy (0.25, 0.5 and 0.75 wt%). The introduction of the aluminium alloy powder has been made in order to improve the mechanical properties, evaluated as the transverse rupture strength, without decreasing the magnetic properties (evaluated in terms of iron loss and coercivity force). The fracture analysis of investigated systems puts into evidence the breaking of interparticle neck connections. Heat treatment (at the temperature of 500 ◦C) contributes to the early stages of interparticle neck developments. The chosen aluminium alloy presents a sort of pre-sintering behaviour at 500 ◦C, with the possibility of mass-transport processes around the insulated iron powder compounds. The air heat treatment applied aims at providing an increase in the mechanical behaviour of the material, with a nal good rigidity after the cooling process. Fracture surfaces and transverse rupture strength values show that, at 500 MPa, the strength and the area related to the inter-particle necks can be correlated to the occasional broken insulated point-to-point surfaces that hinder the development of inter-particles necks. DOI: 10.12693/APhysPolA.128.647 PACS: 75.50.y, 81.20.Ev, 81.40.Np Results obtained in  show that a maximum tem- 1. Introduction ◦ Iron insulated powder compounds (IIPC) represent a relatively new material to be used in electrical machines and further design, material and manufacturing development. According to , the application of insulated powders to form magnetic cores for electric motors operating at low frequencies met with limited success. Nowadays, a successful design requires new thinking, a laminated component that is replaced with an exact replica made of iron powder. The ideal soft magnetic material is an isotropic media with very high magnetic permeability, low coercivity and high saturation induction. In addi- tion, the material should be easily shaped into 3D structures in order to fully take advantage of the material's isotropic nature . Lemieux et al.  underline that for induction machines with very low air gaps, operating at regular power frequencies (5060 Hz), and for highpower-density machines, the poor properties of powdered materials with high hysteresis losses are barely acceptable. In addition, their mechanical strength is very low (maximum 100 MPa). perature of about 500 C is compatible with the conservation of good magnetic properties of IIPC: the attention has then been devoted to select a material able to introduce mechanical advantages under heat treatment at the reported temperature. Dierent powders have been mixed, the insulated iron powder (IIPC) and an AlMg SiCu alloy (as the additional element), this latter responsible for the more homogeneous microstructure and as a better plastically ability agent than matrix powder one. The details about the role of aluminium based alloy in iron based SMC on magnetic materials, as well as the comparison of the properties of investigated materials with original SMC are presented in . Insulated than iron powders laminations 400 Hz [2, 6, 12]. at tend to perform frequencies However, higher better than for low frequency AC soft magnetic applications, the materials must have high permeability, low core losses and acceptable mechanical strength to compete with steel laminated assemblies. 2. Experimental conditions This issue severely limits their elds of application. steel The IIPC material (Somaloy 1P 700, Höganäs AB) has been blended with dierent amounts of aluminium alloy (ready-to-press aluminium based powder Alumix 321: Al0.95 wt% Mg0.49 wt% Si0.21 wt% Cu0.07 wt% * corresponding author; e-mail: [email protected] Fe1.6 wt% lubricant, Ecka Granules). The investigated systems are given in the Table. (647) 648 R. Bidulský et al. TABLE the basic failure mechanism is the interparticle ductile The investigated systems. fracture. A distinct case of interparticle failure is the separation along the original particle surfaces without or System Chemical composition A IIPC + 0.25% Alumix 321 B IIPC + 0.5% Alumix 321 IIPC + 0.75% Alumix 321 C with only minimal local plastic ow . The presence of oxides along the grain boundaries in particle connections results in an interparticle intergranular failure. Transparticle transgranular ductile failure of sintered microstructure occurs only in the case of a low-porous and high- Powder mixtures (PM) were homogenized using a laboratory Turbula mixer for 20 min. Specimens with a dierent green density obtained using a 2000 kN hydraulic press, in a disc-shaped mould (Φ40 mm) and unnotched impact energy 55 × 10 × 10 3 mm specimens ap- plastic matrix. When transgranular cleavage fracture develops in sintered steels it has a transparticle character. In a highly porous microstructure it may transform into interparticle ductile failure . As shown in Figs. 13, a low level of sinter necks plying a pressure in the range 200, 300, 400, 500, 600 was reached after heat treatment. and 700 MPa. dence of major plastic strains at the interparticle necks. Thermal treatments in air at the maxi- There was no evi- ◦ mum temperature of 500 C for 30 min were carried out on the evaluated systems. The green compacts were weighed with an accuracy of ±0.001 g. The dimensions were measured with a micrometer calliper (±0.01 mm). Densities were evaluated using the water displacement method (the Archimede principle), according to the ASTM B96208 standard. The three-point bending (transverse rupture strength, TRS) test is based on the deformation of the specimen by bending with slow force until the moment when material failure occurs in the area of tension/stress. Surface chemical analysis of the powder surface was performed by means of X-ray photoelectron spectroscopy using a PHI 5500 instrument. X-ray photoelectron spec- Fig. 1. Fracture surface of system A. troscopy was used in order to identify elements, present on the powder surface, together with their chemical state. The analyzed area during XPS analysis was about 0.8 mm in diameter and thus a large number of particles (more than 100 particles) was analyzed at the same time giving a statistically reliable average result that represents the general powder surface composition. Determination of the surface oxide layer thickness and compositional proles was done by altering of ion etching and + XPS analysis. The ion etching was performed by Ar gas with an accelerating voltage of 4 kV to the depths of 1, + beam was rastered on the area 2 −1 mm with an etching rate of 25 nm min . 16 and 50 nm. The Ar from 4×5 Fracture surfaces were investigated by means of Fig. 2. Fracture surface of system B. SEM JEOL 7000F. 3. Results and discussion The existence of free internal surfaces in sintered microstructure, such as pores and/or particle connections, results in several specic failure mechanisms. The fracture surfaces of PM materials are dierent from those observed on specimens made by other processes due to the interior pore surfaces. Some authors documented  that the fraction of pore edges, which appear as smooth free particle surfaces, varies with density, where lowdensity regions display large amounts of these free surfaces. In a highly porous and suciently plastic matrix, Fig. 3. Fracture surface of system C. Interparticle Neck Connections in Innovative 649 Insulated Iron Powder Compounds In addition, well-dened insulated surfaces were present in the systems close to the areas where secondary porosity was present. Strength properties, evaluated in terms of TRS values, are reported in the following Fig. 4. Fig. 6. Apparent atomic concentration proles of the fracture surfaces of systems A at 500 MPa. Fig. 4. Strength properties represent by TRS values in MPa. Fig. 7. As in Fig. 6, but for systems B at 500 MPa. The chosen aluminium alloy presents a sort of pre- ◦ sintering behaviour at 500 C, with the possibility of Fig. 5. Iron signal acquired with XPS from the fracture surfaces of systems A, B and C at 500 MPa. mass-transport processes around the insulated iron parti- Some treatment. viding an increase in the mechanical behaviour of the ma- These bonds are formed by thermal oxidation during the terial, with a nal good rigidity after the cooling process. bonds heat treatment. were created during heat It is well known that heat treatment has to develop interparticle bonds, homogeneous distribution of aluminium alloying elements, and a reduction in ◦ porosity. Heat treatment (at the temperature of 500 C) contributes to the early stages of interparticle neck developments. According to [16, 17] this phenomenon revealed cles, whereas the air heat treatment applied aims at pro- Fracture surfaces and TRS values show interparticle necks can be correlated to the occasional broken insulated point-to-point surfaces that hinder the development of interparticles necks. that interparticle oxide bonds formed during a heat treatment at moderate temperature lead to cohesive bonds between iron particles. The breaking points, in terms of strength loss at 300 MPa, are conrmed by the fracture analysis of investigated systems as well as X-ray photoelectron spectroscopy (XPS) analysis. Figure 5 shows that the fracture surface is completely covered by oxides where the main contribution comes from Fe 3+ . Figures 68 present the apparent atomic concentration at dierent etching depths. It can be seen that the main elements are Fe and O. Phosphorous prole is almost identical for the three samples and no aluminium was detected in any of the fracture surfaces, at least with the etching depth that was used. Also, the oxygen content seems to increase from system A to system C. that, at 300 MPa, the strength and the area related to the Fig. 8. As in Fig. 6, but for systems C at 500 MPa. 650 R. Bidulský et al. 4. Conclusions 1. The strength properties of new investigated systems depend on the occasional broken insulated point-to-point surfaces. 2. In terms of fracture, a low level of sinter necks was determined. There was no evidence of major plastic strains at the interparticle necks. 3. Present results, for low frequency AC soft magnetic applications, shows possibility of an AlMgSiCu alloy as the new additional element to the IIPC. Acknowledgments This work was realized within the frame of the Operational Program Research and Development: The centre of competence for industrial research and development in the eld of light metals and composites, project code ITMS: 26220220154 and nancially supported by a European Regional Development Fund. References  P. Lemieux, R. Guthrie, M. Isac, JOM 64, 374 (2012).  H. Shokrollahi, K. Janghorban, J. Mater. Process. Technol. 189, 1 (2007).  C. Gélinas, D. Brydges, SAE Techn. Pap. 2003-010447, (2003).  D. Olek²áková, J. Füzer, P. Kollár, S. Roth, J. Magn. Magn. Mater. 333, 18 (2013).  C. Oikonomou, E. Hryha, L. Nyborg, Surf. Interface Anal. 44, 1166 (2012).  R. Bidulský, M. Actis Grande, L. Ferraris, P. Ferraris, J. Bidulská, Acta Phys. Pol. A 118, 802 (2010).  I.P. Gilbert, V. Moorthy, S.J. Bull, J.T. Evans, A.G. Jack, J. Magn. Magn. Mater. 242-245, 232 (2002).  R. Bidulský, J. Bidulská, M. Actis Grande, L. Ferraris, Acta Metall. Slovaca 20, 271 (2014).  R. Bidulský, M. Actis Grande, L. Ferraris, J. Bidulská, J. Optoelectron. Adv. Mater. 12, 1356 (2010).  J. Bidulská, R. Ko£i²ko, R. Bidulský, M.A. Grande, T. Doni£, M. Martikán, Acta Metall. Slovaca 16, 4 (2010).  M. Actis Grande, R. Bidulsky, A. Cavagnino, L. Ferraris, P. Ferraris, IEEE Trans. Ind. Appl. 48, 1335 (2012).  A.G. Jack, B.C. Mecrow, P.G. Dickinson, D. Stephenson, J.S. Burdess, N. Fawcett, J.T. Evans, IEEE Trans. Ind. Appl. 36, 1077 (2000).  E. Dudrova, M. Kabatova, R. Bidulsky, RoPM 2005, Vol. 1, TU, Cluj-Napoca, 2005, p. 101.  T.F. Murphy, B. Lindsley, Adv. Powder Metall. Particul. Mater. 2, 11 (2007).  E. Dudrova, M. Kabatova, Powder Metall. Progr. 8, 59 (2008).  T. Werber, in: Non-Stoichiometric Compounds Surfaces, Grain Boundaries and Structural Defects, Eds. J. Nowotny, W. Weppner, 1989, p. 547.  L.P. Lefebvre, S. Pelletier, C. Gélinas, Adv. Powder Metall. Particul. Mater. 8, 47 (1998).
© Copyright 2022 Paperzz